A new esthetic fiber-reinforced polymer composite resin archwire: a comparative atomic force microscope (AFM) and field-emission scanning electron microscope (FESEM) study
© Chng et al.; licensee Springer. 2014
Received: 2 January 2014
Accepted: 9 April 2014
Published: 30 May 2014
Fiber-reinforced polymer composite (FRPC) archwires could provide an esthetic solution to conventional orthodontic archwires. This study was carried out with the following aims: (1) to compare the sliding friction of FRPC archwire with nickel titanium archwire using various archwire-bracket combinations and (2) to determine the correlation between surface roughness and friction of the FRPC and NiTi archwires.
Four different brackets (Gemini® (Gemini-3M Unitek, St. Paul, MN, USA), ICE® (ICE-Ormco- Orange, CA, USA), Clarity® (Clarity-3M Unitek, St. Paul, MN, USA), and SmartClip® (SmartClip-3M Unitek, St. Paul, MN, USA)) in combination with FRPC wires and NiTi wires (0.018 in) were studied for archwire friction with simulated wear and surface roughness using scanning electron microscope (SEM) and atomic force microscope (AFM), respectively. Statistical analysis of frictional wear generated and surface roughness between the various archwire and bracket groups was evaluated by one-way ANOVA at 5% level. Least significant difference (LSD) multiple comparisons were used to determine the archwire-bracket group difference.
Gemini®-FRPC group generated the highest frictional wear (mean, 313.10; SD, 802.59) and ICE®-FRPC group produced the highest roughness values among all the groups tested (Ra = 496.13 nm, RMS = 635.49 nm). No correlation was found between frictional wear and surface roughness of the archwires of the various groups.
FRPC archwire shows promise in its application as an esthetic aligning archwire. However, further research and refinement in its manufacture would be necessary to fully realize its potential as an esthetic archwire.
With the advent of increasing number of adults opting for orthodontic treatment, the development of orthodontic appliances with ample emphasis on esthetics coupled with optimal performance has become an exceedingly essential goal or rather necessity of the day. Through composite technology, an esthetic wire has been developed from continuous fibers (E-glass fiber) and epoxy polymer matrix (tube shrinkage technique), giving rise to a prototype, fiber-reinforced polymer composite (FRPC) archwire (BioMers Products LLC, Naples, FL, USA), which is potentially suitable for use in orthodontics . Literature suggests that the bending stiffness and strength of the FRPC archwire were comparable to those archwires routinely used in orthodontic treatment [2–4].
Springback, stiffness, formability, resilience modulus, biocompatibility, and low friction are some of the desirable characteristics of an archwire for optimum mechanical performance during orthodontic treatment [5, 6]. FRPC archwire's tensile and three-point bending tests have shown that the archwire's mechanical properties are comparable to nickel titanium .
In the past, coated esthetic wires have been used as archwires, fixed retainers , and to reinforce anchorage , but such wires have higher friction (archwires), and the esthetic coating tend to dehisce over a period of time [9–17]. Also, coated wires, being opaque, cause no tooth color transmission through these wires. The FRPC archwire, being translucent in nature, allows tooth color transmission, thereby improving esthetics. Aforementioned phenomenon is particularly beneficial in cases where ceramic/tooth colored brackets are used in conjunction with FRPC wires for orthodontic treatment. Moreover, allergic reactions to nickel [18–21], a metallic ion found commonly in contemporary metallic archwires, is averted with the FRPC archwire.
Although, FRPC can offset the unpleasant appearance of the metallic archwires, the frictional characteristics of the wire cannot be overlooked, as friction plays a critical role throughout the course of orthodontic treatment [22, 23]. At various stages of orthodontic treatment, the mechanical properties required by the archwire differ; different fiber material, fiber content, and fiber arrangement can modify the mechanical properties of the wire to suit the mechanical requirements of the archwire at various stages of treatment.
Moreover, low friction is one of the optimal desirable properties of an ideal orthodontic archwire [24, 25]. The success or failure of fixed appliance orthodontic treatment is greatly influenced by the frictional properties of the materials used and how friction is applied and controlled, in the due course of treatment.
to determine sliding friction of FRPC archwire with nickel titanium archwire using various archwire-bracket combinations
to determine the correlation between surface roughness and friction of the FRPC and NiTi archwires.
Therefore, the null hypothesis tested was that there would be no difference in sliding friction and surface roughness of FRPC archwire and nickel titanium archwires when combined with different bracket systems.
Brands, manufacturing companies, configurations, and composition of various brackets used in this study
3M Unitek, St. Paul, MN, USA
3M Unitek, St Paul, MN, USA
Polycrystalline metal-reinforced ceramic
Ormco, Orange, CA, USA
3M Unitek, St Paul, MN, USA
Orthodontic archwires used in the study
Wire size (in.) and brand
Mixture of cured copolymers, Bis-EMA, TEGDMA, and glass fibers
BioMers Products LLC, Naples, FL, USA
52% Ni, 45% Ti, and 3% Co
International Orthodontic Services Inc., Houston, TX, USA
Five tests were carried out for each bracket and archwire combination. A total of eight archwire and bracket combinations were formed with two archwires and four different brackets. The values of the frictional wear of each archwire-bracket test were captured from the universal testing machine to dedicated software (Merlin Software, Instron Corporation); this software was used to calculate the frictional values. Field emission scanning electron microscope (FESEM) and atomic force microscope (AFM) studies were conducted for qualitative surface analysis and quantitative analysis of the archwires, respectively.
The scanning electron microscope (SEM) study was carried out with a field-emission scanning electron microscope (FESEM) (Quanta 200F, FEI, Hillsboro, OR, USA). One test wire from each of the wire-bracket combination was used for the FESEM analysis. One untested FRPC wire and one untested NiTi wire from each group formed the control sample. Before subjecting the specimens for FESEM analysis, all the specimens were prepared by placing them individually into an auto fine coater (JEOL Model JFC 1600, Tokyo, Japan). The samples were gold coated for 60 s using a 10-mA current. The area for FESEM scanning was localized by determining the middle of the friction test site and the area 1 mm above and below this mid-point along which the length of the wire was scanned. This area was scanned and analyzed with magnification factor of ×220 to ×5,000.
AFM (Dimension™ 3100, Nanoscope IIIa, Digital Instruments Inc., Santa Barbara, CA, USA) with ‘RTESP Tap300’ Metrology Probe (Veeco, Plainview, NY, USA) was used to perform the surface analysis of the archwires in this study. The microscope raster scans were obtained by placing the probe over the sample while measuring the local properties (height, optical absorption, and magnetism). Tapping Mode™ (Nanocsope IIIa, Digital Instruments Inc.) was used to analyze the surface topography of the test wires. For the purpose of comparison, the root mean square (RMS) roughness was chosen to characterize the topography of the test wires after the test wires have undergone frictional testing with the universal testing machine. For AFM analysis, four test wire-bracket combinations were randomly selected from the original sample of five test wire and bracket combinations. The 1-mm test area created by universal testing machine was visually scanned and localized using the nanoscope, and three surface scans were taken from the area: one at the middle and two more at the ends of the test area. The RMS roughness of these surface areas was determined along with mean and standard deviation .
All the statistical analyses were carried out using the statistical package for social sciences (SPSS version 14, SPSS Inc., Chicago, IL, USA) software. Based on the preliminary data and a test power analysis of 0.85, the sample size calculation showed that at least three specimens are sufficient to detect a 10% difference with a significance level of 5%. The mean and standard deviation of the frictional wear and surface roughness were evaluated. A one-way ANOVA was carried out to compare the friction wear and surface roughness between groups and also within groups. Multiple comparisons were performed using least significant difference (LSD) with a post hoc Bonferroni adjustment.
Quantitative analysis of friction study
Descriptive statistics of eight bracket-archwire combinations tested for friction and roughness (AFM)
(mean ± SD)
(mean ± SD)
−27.88 ± 33.59
324.96 ± 143.76
−22.83 ± 34.74
166.88 ± 39.66
313.10 ± 802.59
310.45 ± 70.46
75.41 ± 159.06
183.95 ± 44.53
−71.13 ± 17.08
398.47 ± 249.04
−28.48 ± 21.44
206.55 ± 70.74
27.48 ± 72.85
321.16 ± 27.52
−6.94 ± 48.27
172.80 ± 52.49
There was no significant difference noted for the frictional wear generated between the various archwire and bracket groups (P = 0.542). Also, no statistical significance was noted within individual archwire-bracket groups (Table 3).
Multiple comparisons of the groups showed significant difference in frictional wear. LSD multiple comparison revealed statistical significance (P < 0.05) when comparing the Gemini-FRPC with the ICE-FRPC group. No other groups showed any significant difference.
Qualitative analysis of SEM study
Control FRPC and NiTi wires
Both FRPC and NiTi control wires appeared to be relatively smooth with minimal surface defects. Inclusions noted on surfaces were probably not inherent of the surface structures, but could be a result of contamination during handling of these wires.
Tested NiTi wires
Tested FRPC wires
Quantitative analysis of surface roughness from AFM study
The surface roughness values were generally higher in bracket-archwire combinations with the FRPC archwire. The ICE-FRPC group produced the highest roughness values among all the groups tested. Untested wires were also analyzed for roughness, where untested FRPC showed average roughness of RMS = 321.89 nm and untested NiTi wires showed roughness of RMS = 261.5689 nm.
The null hypothesis of the study was rejected as different archwire-bracket combinations produced different degrees of surface roughness, with the ICE-FRPC group showing the highest roughness value among all the groups tested (Table 3). The FRPC wire tested in this study has been designed and manufactured with the intention to function as wire used in the initial alignment phase of orthodontic treatment with high esthetic value. The use of equivalent-diameter contemporary nickel titanium archwires for comparison of friction and surface roughness is therefore appropriate. Four different brackets and two archwire materials were combined to give eight different bracket-archwire interface combinations to quantify the amount of sliding friction and surface roughness with SEM and AFM, respectively. The wear patterns created on the surface of each archwire material with the eight different bracket-archwire interfaces were determined and were co-related with the sliding friction and surface roughness.
Frictional wear from the friction studies showed no significant difference between the groups. From the LSD multiple comparison, only the ICE-FRPC group showed statistical significance when compared to the Gemini-FRPC group. However, a post hoc Bonferroni adjustment for multiple comparisons showed that the Gemini-FRPC group showed no statistical significance. All other FRPC combination groups did not show any statistical significance in the frictional testing. This would indicate that the FRPC wire's performance was similar to that of the NiTi wire during friction testing.
Scanning electron microscopy of surface wear
Clarity bracket (ceramic) and wire combination showed crystal-like structural deposits on the tested wires. However, the same was not noted in ICE (ceramic) bracket-wire combination. Though both (Clarity and ICE) are ceramic brackets, the structural deposits were not noted in the ICE bracket-wire combination; this could be attributed to the structural differences in both brackets. Clarity is polycrystalline and ICE is monocrystalline; polycrystalline ceramic brackets usually have structural imperfections, and the incorporation of impurities as a result of manufacturing process makes it structurally weaker than monocrystalline ceramic brackets . Microfractures may also have occurred in the Clarity bracket, giving rise to fragments of deposits on the surface of the tested wires. All the tested bracket slots were reobserved for asperities arising as a result of wire abrasion and also observed for bracket slot color changes arising from the metallic wire. Neither asperities nor color changes were noted, confirming the fragments of deposits to be bracket microfractures.
NiTi wires showed horizontal wear tracks; these finding were congruent with the findings noted by Al-Khatib et al. . Scratches, groves, and oxidized layer were noted which are believed to be caused by the wear mechanisms that are active in the sliding contacts between the bracket and archwire, inducing a competition between abrasive wear and oxidational wear processes. Along with the aforementioned findings, vertical track marks were also noticed which could be due to the result of ligation of the wire with stainless steel ligation wires.
FRPC wires also appeared to have fibers exposed after frictional testing. The exposure of the fibers did not significantly affect roughness or frictional values. Discrete penetration separated by sections of undamaged coating was observed in one of the wires. This was also noted by Zufall et al. . The cause of the bulk fracture of composite is yet to be ascertained, but a likely reason would be an area of weakness due to premature polymerization of the composite during the manufacturing process or a void that was present just below the area of penetration.
Atomic force microscopy of surface roughness
A commercial AFM (Dimension 3100, Nanocsope IIIa, Digital Instruments Inc.) was used to perform the surface analysis of the archwires. The AFM is one of the types of scanned-proximity probe microscopes (SPMs). The tip used in this study was the RTESP Tap300 Metrology Probe. SPMs work by measuring a local property, such as height, optical absorption, and magnetism, with a ‘probe’ or ‘tip’ placed very close to the sample. The small probe-sample separation (on the order of the instrument's resolution) makes it possible to take measurements over a small area. To acquire an image, the microscope raster scans the probe over the sample while measuring the local property in question. The resulting image resembles an image on a television screen in that both consist of many rows or lines of information placed one above the other.
Unlike traditional microscopes, scanned-probe systems do not use lenses; hence, the size of the probe rather than diffraction affects the resolution. The tip is very fine (<100 nm) and is mounted on a thin cantilever of approximately 100 μm in length. The cantilever has a deflection modulus between 0.001 and 100 N/m, bringing the tip into a distance of about 10 to 100 nm of the specimen surface. This interaction between specimen surface and tip results in forces that range between 10−11 and 10−6 N. Due to this interaction, the cantilever was bent, and the vertical deflection of its end was registered by a deflection sensor. The AFM thus operates by measuring attractive or repulsive forces between the tip and the sample. There are many modes of scanning that can be used by the AFM. The three most common are the (1) contact, (2) non-contact, and (3) Tapping Mode™. Tapping Mode™ AFM, the most commonly used of all AFM modes, is a technique that maps topography by lightly tapping the surface with an oscillating probe tip. The cantilever's oscillation amplitude changes with sample surface topography, and the topography image is obtained by monitoring these changes and closing the z feedback loop to minimize them. TappingMode™ has become an important AFM technique, as it overcomes some of the limitations of both contact and non-contact AFM. By eliminating lateral forces that can damage soft samples and also reduce image resolution, TappingMode™ allows routine imaging of samples once considered impossible to image with AFM, especially in contact mode. Another major advantage of Tapping Mode™ is related to the limitations that can arise due to the thin layer of liquid that forms on most sample surfaces in an ambient imaging environment, i.e., in air or some other gas. The amplitude of the cantilever oscillation in TappingMode™ is typically on the order of a few tens of nanometers, which ensures that the tip does not get stuck in this liquid layer. The amplitude used in non-contact AFM is much smaller, as different forces are being measured. As a result, the non-contact tip often gets stuck in the liquid layer unless the scan is performed at a very slow speed. In general, TappingMode™ is much more effective than non-contact AFM for imaging larger scan sizes that may include large variations in sample topography. TappingMode™ can be performed in gases, liquids, and some vacuum environments. For this part of the study using the AFM, the TappingMode™ was used to analyze surface topography of the test wires.
RMS roughness was chosen to characterize the topography of the test wires. Roughness is a generic term that is used to indicate unevenness, whereas RMS is a quadratic mean, a statistical measure of the magnitude of a varying quantity. It is especially useful when variants are positive and negative and are taken from a sample surface, but not from the entire surface. In our study, the peak and valley on the sample surface measured indicates the positive and negative variants. Hence, RMS was used to measure a sample of peaks and valleys.
There was a significant difference noted for the roughness between the various archwire and bracket groups (P = 0.044). However, no statistical significance was evident within individual groups.
The ICE-FRPC group had the highest roughness value among all the groups tested. ICE, being a monocrystalline ceramic bracket, is manufactured by milling and is very hard . The milling process produces sharp corners; this, coupled with hardness, is likely to cause surface roughness on the FRPC wire.
The average roughness of the untested FRPC wire and NiTi wire was also analyzed with the AFM. There was no statistical difference between the untested FRPC and untested archwires.
For all groups tested for surface roughness, surface roughness was significantly higher in ICE-FRCP when compared to the groups with NiTi wire. This can be attributed to the higher hardness value of ICE. Further investigations is essential to validate this finding, as it is highly probable that FRPC archwires will likely be used with some form of ceramic bracket in clinical scenarios.
The relationship between sliding friction and surface roughness
There was no correlation that could be drawn from the frictional wear and surface roughness. A higher frictional value did not translate to higher roughness values. Aforementioned observations are anticipatory and are in agreement with various studies previously carried out [25–30]. This could be attributed to many reasons; one reason could be the type of ligation. Although the type of ligation was standardized using stainless steel ligatures, it could have been more uniformed, if a steady and predictable force system could be applied via a customized jig and load cell. This arrangement would have ensured uniform seating forces of the archwire into the bracket for all the samples.
FRPC wires are a mixture of cured copolymers (Bis-EMA, TEGDMA, and glass fibers) (Table 2). Intraoral dissolution or leaching out of polymer from the composite wires might pose a potential health issue. Our study revealed exposure of fibers after frictional testing; hence, the concern would be if the wearing off of the polymer composite into the oral cavity would lead to any potential health-related issues [4, 24, 30]. Increased plaque accumulation and slow tooth movement (increased archwire-bracket friction) might be a possibility due to formation of irregular surface at fiber-exposed sites.
FRPC archwires are still in its infancy of development. Future directions in experimentation would be to include a fluid medium, like saliva, to compare wet and dry states of friction involving various orthodontic bends. Given the fact that composite wires stain easily, future focus should be on the staining characteristics of these composites wires with different beverages consumed during the course of the orthodontic treatment.
Based on the discussion above, the following conclusions were drawn:
FRPC and NiTi wires show statistically comparable frictional wear when used with ICE, Gemini, Clarity, and SmartClip brackets.
Different archwire-bracket combinations produced different degrees of surface roughness.
No correlation was found between frictional wear and surface roughness of the archwires of the various groups.
FRPC wire has the potential to be used as an esthetic orthodontic archwire during the alignment stage. This is based on the comparable frictional wear and surface wear results as observed in this study.
- Huang Z-M, Gopal R, Fujihara K, Ramakrishna S, Loh PL, Foong WC, Ganesh VK, Chew CL: Fabrication of a new composite orthodontic archwire and validation by a bridging micromechanics model. Biomaterials 2003, 24: 2941–2953. 10.1016/S0142-9612(03)00093-0View ArticlePubMedGoogle Scholar
- Fallis DW, Kusy RP: Variation in flexural properties of photo-pultruded composite archwires: analyses of round and rectangular profiles. J Mater Sci Mater Med 2000, 11: 683–93. 10.1023/A:1008903224180View ArticlePubMedGoogle Scholar
- Karmaker AC, DiBenedetto AT, Goldberg AJ: Continuous fiber reinforced composite materials as alternatives for metal alloys used for dental applications. J Biomater Appl 1997, 11(3):318–28.PubMedGoogle Scholar
- Jancar J, Dibenedetto AT, Hadziinikolau Y, Goldberg AJ, Dianselmo A: Measurement of the elastic modulus of fiber-reinforced composites used as orthodontic wires. J Mater Sci Mater Med 1994, 5: 214–8. 10.1007/BF00121091View ArticleGoogle Scholar
- Kusy RP: Influence of force systems on archwire-bracket combinations. Am J Orthod Dentofacial Orthop 2005, 127(3):333–42. 10.1016/j.ajodo.2004.07.037View ArticlePubMedGoogle Scholar
- Salehi P, Najafi HZ, Roeinpeikar SM: Comparison of survival time between two types of orthodontic fixed retainer: a prospective randomized clinical trial. Prog Orthod 2013, 14: 25. 10.1186/2196-1042-14-25PubMed CentralView ArticlePubMedGoogle Scholar
- Pizzoni L: Fibre reinforced composite transpalatal arch in impacted canine orthodontic treatment. Prog Orthod 2010, 11(1):83–5. 10.1016/j.pio.2010.04.011View ArticlePubMedGoogle Scholar
- Kusy RP, Whitley JQ, Prewitt MJ, Kusy RP, Whitley JQ, Prewitt MJ: Comparison of the frictional coefficients for selected archwire-bracket slot combinations in the dry and wet states. Angle Orthod 1991, 61(4):293–302. Erratum in: Angle Orthod. 1993, 63(3):164 Erratum in: Angle Orthod. 1993, 63(3):164PubMedGoogle Scholar
- Zufall SW, Kennedy KC, Kusy RP: Frictional characteristics of composite orthodontic archwires against stainless steel and ceramic brackets in the passive and active configurations. J Mater Sci Mater Med 1998, 9(11):611–20. 10.1023/A:1008977106648View ArticlePubMedGoogle Scholar
- Ohtonen J, Vallittu PK, Lassila LVJ: Effect of monomer composition of polymer matrix on flexural properties of glass fibre-reinforced orthodontic archwire. Eur J Orthod 2013, 35: 110–114. 10.1093/ejo/cjr128View ArticlePubMedGoogle Scholar
- Elayyan F, Silikas N, Bearn D: Ex vivo surface and mechanical properties of coated orthodontic archwires. Eur J Orthod 2008, 30: 661–667. 10.1093/ejo/cjn057View ArticlePubMedGoogle Scholar
- Elayyan F, Silikas N, Bearn D: Mechanical properties of coated superelastic archwires in conventional and self-ligating orthodontic brackets. Am J Orthod Dentofacial Orthop 2010, 137: 213–7. 10.1016/j.ajodo.2008.01.026View ArticlePubMedGoogle Scholar
- Cacciafesta V, Sfondrini MF, Alessandro L, Scribante A, Vallittu PK, Lassila LV: Force levels of fiber-reinforced composites ad orthodontic stainless steel wires: a 3-point bending test. Am J Orthod Dentofacial Orthop 2008, 133: 410–413. 10.1016/j.ajodo.2006.01.047View ArticlePubMedGoogle Scholar
- Kusy RP, Whitley JQ: Effects of surface roughness on the coefficients of friction in model orthodontic systems. Journal of Biomechanics 1990, 23: 913–925. 10.1016/0021-9290(90)90356-8View ArticlePubMedGoogle Scholar
- Corbitt GV: Commentary: reduced frictional resistances using Teflon-coated ligatures with various bracket-archwire combinations. The Angle Orthodontist 1995, 65: 73–74.Google Scholar
- Pamela H, Christoph B, Michael W, Andreas J: The frictional behavior of coated guiding archwires. J Orofac Orthop 2002, V63: 199–211.Google Scholar
- Franco DJD, E R, Spiller J, Fraunhofer JA: Frictional resistances using Teflon-coated ligatures with various bracket-archwire combinations. Angle Orthod 1995, 65: 63–74.PubMedGoogle Scholar
- Al-Khatib S, Berradja A, Celis JP, Willems G: In vitro friction of stainless steel archwire-bracket combinations in air and different aqueous solutions. Orthod Craniofac Res 2005, 8: 96–105. 10.1111/j.1601-6343.2005.00321.xView ArticlePubMedGoogle Scholar
- David A, Lobner D: In vitro cytotoxicity of orthodontic archwires in cortical cell cultures. Eur J Orthod 2004, 26: 421–426. 10.1093/ejo/26.4.421View ArticlePubMedGoogle Scholar
- Eliades T, Bourauel C: Intraoral aging of orthodontic materials: the picture we miss and its clinical relevance. Am J Orthod Dentofacial Orthop 2005, 127: 403–412. 10.1016/j.ajodo.2004.09.015View ArticlePubMedGoogle Scholar
- Oh K-T, Kim K-N: Ion release and cytotoxicity of stainless steel wires. Eur J Orthod 2005, 27: 533–540. 10.1093/ejo/cji047View ArticlePubMedGoogle Scholar
- Nishio C, da Motta AFJ, Elias CN, Mucha JN: In vitro evaluation of frictional forces between archwires and ceramic brackets. Am J Orthod Dentofacial Orthop 2004, 125: 56–64. 10.1016/j.ajodo.2003.01.005View ArticlePubMedGoogle Scholar
- Smart FM: Kinetic friction. Am J Orthod Dentofacial Orthop 2004, 125: A17–17. 10.1016/j.ajodo.2003.11.013View ArticleGoogle Scholar
- Clocheret K, Willems G, Carels C, Celis JP: Dynamic frictional behaviour of orthodontic archwires and brackets. Eur J Orthod 2004, 26: 163–170. 10.1093/ejo/26.2.163View ArticlePubMedGoogle Scholar
- Kusy RP, Whitley JQ: Resistance to sliding of orthodontic appliances in the dry and wet states: influence of archwire alloy, interbracket distance, and bracket engagement. J Biomed Mater Res 2000, 52(4):797–811. 10.1002/1097-4636(20001215)52:4<797::AID-JBM25>3.0.CO;2-9View ArticlePubMedGoogle Scholar
- Bishara SE, Fehr DE: Ceramic brackets: something old, something new, a review. Semin Orthod 1997, 3: 178–188. 10.1016/S1073-8746(97)80068-0View ArticlePubMedGoogle Scholar
- Bourauel C, Fries T, Drescher D, Plietsch R: Surface roughness of orthodontic wires via atomic force microscope, laser specular reflectance, and profilometry. Eur J Orthod 1998, 20: 79–92. 10.1093/ejo/20.1.79View ArticlePubMedGoogle Scholar
- Eliades T, Eliades G, Brantley WA, Johnston WM: Residual monomer leaching from chemically cured and visible light-cured orthodontic adhesives. Am J Orthod Dentofacial Orthop 1995, 108: 316–321. 10.1016/S0889-5406(95)70027-7View ArticlePubMedGoogle Scholar
- Kusy RP, Whitley JQ: Effects of sliding velocity on the coefficients of friction in a model orthodontic system. Dental Materials 1989, 5: 235–240. 10.1016/0109-5641(89)90067-5View ArticlePubMedGoogle Scholar
- Eliades T, Pratsinis H, Kletsas D, Eliades G, Makou M: Characterization and cytotoxicity of ions released from stainless steel and nickel-titanium orthodontic alloys. Am J Orthod Dentofacial Orthop 2004, 125: 24–29. 10.1016/j.ajodo.2003.09.009View ArticlePubMedGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.